conductive polymers or , more precisely , intrinsically conducting polymers are organic polymers that conduct electricity , and such compounds may have metallic conductivity or can be semiconductors . some of the well - studied organic conductive polymers , according to their composition , are polyaniline , polypyrrole , polythiophene , polyacetylene , poly(p - phenylene vinylene ) , poly(p - phenylene sulfide ) , and polycarbazole . polycarbazole ( pcz ) and its derivatives , which have a structure of pyrrole ring with two fused benzene rings , are well known to exhibit good electroactive and photoactive properties . pcz is being explored for various applications especially in hole transporting and photoluminescence efficiency , electroluminescence [ 35 ] , light - emitting diodes , electrochromic displays , supercapacitor , chemical batteries [ 9 , 10 ] , sensors [ 11 , 12 ] , and laser dyes and organic transistors . studies on polycarbazole and its derivatives synthesized by electrochemical method have been reported [ 1417 ] . however , work on chemical synthesis of unsubstituted carbazole is very few , even though chemical synthesis for substituted polycarbazole had already been reported [ 1820 ] . chemical synthesis of pcz is drawing keen attention due to its obvious advantage in morphology control and bulk synthesis . in 2010 , first report of chemical synthesis of unsubstituted pcz in hollow microspheres morphology was reported by gupta and prakash   and raj et al . , that is , the synthesis of soluble pcz by the chemical oxidative polymerization of carbazole using ammonium persulfate in acetonitrile medium . recently , pcz - au composite was synthesized by the oxidation of carbazole using haucl4 oxidant . there is a restriction on the selection of the oxidizing agents due to nonsolubility of oxidizing agents and monomers in the same solvent . since carbazole is not soluble in water and soluble in chloroform , carbazole was oxidized using chloroform soluble benzoyl peroxide oxidant by solution polymerization pathway . also , carbazole was polymerized to polycarbazole , that is , emulsion polymerization pathway using sodium lauryl sulfate as emulsifier . powder of polycarbazole was pressed into a disk of 13  mm diameter and about 1.5  mm thickness under a pressure of 120  kg / cm . resistance of the pellet was measured by two - probe method using 2010 digital multimeter ( keithley , cleveland , ohio , usa ) . the conductivity of the pellet was calculated by the formula  = l/(ar ) , where , l = thickness of the pellet in cm , a = area of the pellet in cm , and r = resistance of the pellet in . pellet density was measured from mass per unit volume of the pressed pellet using the formula d = m/(rl ) , where l = thickness of the pellet in cm and m = mass of the pellet in g. molecular weight of polycarbazole was carried out using maldi - tof - ms instrument ( shimadzu biotech axima performance 2.9.3.20110624 : model linear , power : 80 , blanked , p. ext@4300 ( bin 97 ) uk ) using -cyano 4-hydroxy cinnamic acid matrix . ft - ir spectra of polymer samples were registered on a ft - ir spectrometer ( thermo nicolet nexus 670 , usa ) using the kbr pressed pellet technique . x - ray diffraction profiles for polymer powders were obtained on a siemens / d-500 x - ray diffractometer , usa , using cu k radiation and scan speed of 0.045/min . morphology studies ( microstructural and elemental analyses ) of the polymer samples were carried out with a hitachi s-4300 fe - sem ( tokyo , japan ) . the sample was mounted on a carbon disc with the help of double - sided adhesive tape and sputter - coated with a thin layer of gold to prevent sample charging problems . thermogravimetric analyses of polymer samples were carried out using ta instruments ( tga q500 v20.8 , usa ) from ambient to 700c under nitrogen atmosphere at a heating rate of 10c per minute . cyclic voltammetry experiment was carried with a wonatech multichannel potentiostat / galvanostat ( wmpg 1000 , gyeonggi - do , korea ) . in a typical polymerization system , carbazole ( 1.67  g , 0.1  m ) , and p - toluene sulfonic acid ( 3.8  g , 0.2  m ) were dissolved in 50  ml of chloroform and magnetically stirred for 30  min . to this solution , 50  ml of chloroform solution containing benzoyl peroxide ( 3.6  g , 0.24  m ) was added as a whole . the mixture was stirred constantly for 4  h at an ambient temperature and then precipitated with methanol . the green precipitate was filtered and washed several times with distilled water followed by methanol . the powder sample was dried at 50c in an oven until a constant weight . in a typical polymerization system , carbazole ( 1.67  g , 0.1  m ) was dissolved in 50  ml of chloroform . 25  ml aqueous solution containing 3.8  g p - toluene sulfonic acid ( 0.2  m ) was added while stirring the solution . then 25  ml aqueous solution containing 1  g of sls surfactant ( 0.035  m ) was added slowly while stirring which resulted in an emulsion form . to this emulsion , 25  ml chloroform solution containing 3  g of benzoyl peroxide ( 0.1  m ) was introduced . the mixture was stirred constantly for 4  h at an ambient temperature and then precipitated with methanol . the green precipitate was filtered and washed several times with distilled water followed by methanol . polycarbazole ( s - pcz or e - pcz ) was prepared from polycarbazole salt prepared by solution or emulsion polymerization pathway by dedoping process . 0.5  g of polycarbazole salt was stirred in 50  ml of 1  m aq . naoh solution for 4  h and then filtered and washed several times with distilled water followed by methanol . the powder sample was dried at 50c in an oven until a constant weight . 0.5  g of polycarbazole salt was stirred in 50  ml chcl3 solvent for 4  h at an ambient temperature and then filtered and dried . e - pcz - p - tsa and s - pcz - p - tsa salts are almost completely soluble in thf , dmso , and nmp solvents , whereas the solubility of e - pcz - p - tsa and s - pcz - p - tsa in chloroform is found to be 64 and 9  wt% , respectively . e - pcz and s - pcz bases are almost soluble in dmso and nmp . for the first time , benzoyl peroxide is used as an oxidizing agent for the oxidation of carbazole to polycarbazole . polycarbazole was prepared both by solution and emulsion polymerization pathways by oxidizing carbazole using benzoyl peroxide oxidant in the presence of acid and with or without sodium lauryl sulfate emulsifier ( scheme 1 ) . polycarbazole salt was prepared by solution polymerization by changing the concentration of acid , oxidant , and reaction time . the values of yield , conductivity , and densities of polycarbazole salts are reported in table 1 . the observations are as follows.the values of yield , conductivity , and densities of the polycarbazole salts prepared using 0.1 and 0.2  m of p - tsa are found to be nearly the same.similarly , the values of yield , conductivity , and densities of the polycarbazole salts prepared in 4  h are found to be nearly the same with the sample prepared in 8  h. however , the value of yield increases , that of conductivity decreases , and that of density is found to be the same in 24  h in comparison with 8  h.the values of yield and conductivities of the polycarbazole salts increase with increase in the concentration of the oxidizing agent and the values decrease on further increase in concentration of oxidizing agent.pellet density of polycarbazole salts is found to be the same ( 1.11 to 1.18  g / cm)maximum yield ( 69% ) and conductivity ( 1.5  10  s / cm ) of the polycarbazole salt were obtained with the reaction condition such as carbazole ( 0.1  m ) , p - tsa ( 0.2  m ) , bpo ( 0.12  m ) , and reaction time : 4  h.for comparison , polycarbazole salt was also prepared by emulsion polymerization pathway using aqueous / nonaqueous media in presence of sodium lauryl sulfate surfactant . yield of polycarbazole salt prepared by emulsion polymerization pathway using 0.2  m p - tsa protonic acid ( 60% ) is found to be slightly higher than that of 1  m hcl ( 55% ) used . densities and conductivities of the polycarbazole salts could not be measured because of the course nature of the samples , which in turn did not give pellet . the values of yield , conductivity , and densities of the polycarbazole salts prepared using 0.1 and 0.2  m of p - tsa are found to be nearly the same . similarly , the values of yield , conductivity , and densities of the polycarbazole salts prepared in 4  h are found to be nearly the same with the sample prepared in 8  h. however , the value of yield increases , that of conductivity decreases , and that of density is found to be the same in 24  h in comparison with 8  h. the values of yield and conductivities of the polycarbazole salts increase with increase in the concentration of the oxidizing agent and the values decrease on further increase in concentration of oxidizing agent . pellet density of polycarbazole salts is found to be the same ( 1.11 to 1.18  g / cm ) maximum yield ( 69% ) and conductivity ( 1.5  10  s / cm ) of the polycarbazole salt were obtained with the reaction condition such as carbazole ( 0.1  m ) , p - tsa ( 0.2  m ) , bpo ( 0.12  m ) , and reaction time : 4  h. molecular weight of the polycarbazoles s - pcz - p - tsa and e - pcz - p - tsa was measured by maldi - tof - ms using -cyano 4-hydroxy cinnamic acid matrix and is shown in figures 1(a ) and 1(b ) , respectively . molecular weight of s - pcz - p - tsa and e - pcz - p - tsa was found to be 1655 and 2005 , which corresponds to approximately 10 and 12 monomer units , respectively . however , this molecular weight corresponds only to the soluble part of polymer in thf isolated portion . gupta and prakash reported the molecular weight of polycarbazole prepared by interfacial polymerization method as 1971 ( ~12 monomer units ) from gpc measurement . the infrared spectra of polycarbazole salt and its corresponding base prepared by solution and emulsion polymerization pathways are shown in figures 2 and 3 , respectively . significant observations are as follows.a peak at 2925  cm is observed in all the cases ( both salt and bases ) and this peak may be due to impurities or supertone band or shifted aromatic c  h str . frequency due to the presence of radical on nitrogen atom.a peak at 1730  cm is observed for polycarbazole salts ( e - pcz - p - tsa and s - pcz - p - tsa ) , whereas a small peak is observed fore - pczand no peak for s - pcz . this peak may be often due to -oh from water adduct   or c = o str . due to overoxidation.peaks at 1165 and 1060  cm observed for polycarbazole salts ( e - pcz - p - tsa and s - pcz - p - tsa ) are due to sulfonic group , whereas the peaks almost vanished for polycarbazole bases ( e - pczand s - pcz ) . a peak at 2925  cm is observed in all the cases ( both salt and bases ) and this peak may be due to impurities or supertone band or shifted aromatic c  h str . a peak at 1730  cm is observed for polycarbazole salts ( e - pcz - p - tsa and s - pcz - p - tsa ) , whereas a small peak is observed fore - pczand no peak for s - pcz . this peak may be often due to -oh from water adduct   or c = o str . peaks at 1165 and 1060  cm observed for polycarbazole salts ( e - pcz - p - tsa and s - pcz - p - tsa ) are due to sulfonic group , whereas the peaks almost vanished for polycarbazole bases ( e - pczand s - pcz ) . polycarbazole salt and its corresponding base samples prepared by emulsion polymerization pathway were dissolved in dimethyl sulfoxide and then filtered to get a clear solution . dmso solutions were subjected for uv - vis spectral measurement at ambient temperature . both the salt ( e - pcz - p - tsa ) as well as its base ( e - pcz ) showed one peak at 298 and another shoulder around 350  nm ( figure 4 ) . an absorption band of the polymer at 298  nm corresponds to valance band to conduction band and a shoulder around 350  nm is due to polaron level to  conduction band . these two peaks of the polymer ( 298 & 350  nm ) are different from the monomer peaks of carbazole observed at 289 and 325  nm , respectively . a similar uv - vis spectrum was observed for polycarbazole salt and its corresponding base samples were prepared by solution polymerization pathway . element of sulphur present in pcz systems was qualitatively found out from energy dispersive x - ray spectroscopy . s - pcz - p - tsa ( 1.85% ) and e - pcz - p - tsa ( 1.73% ) , whereas polycarbazole base does not contain sulfur and this result supports the presence of p - tsa as dopant in polycarbazole salt . sem pictures of e - pcz - p - tsa taken at various magnifications are shown in figure 5 . sem image taken at lower magnifications ( figures 5(a ) and 5(b ) ) shows various shapes such as rod , sphere , and pores . in order to find out the length , width , and diameter of various shapes , sem image has been taken at higher magnification ( figures 5(c ) and 5(d ) ) . rod was obtained in 1830  m of length and 2.5  m of width , sphere with 3 to 7  m diameter , and size of the pores 0.6 to 1.1  m . on conversion of e - pcz - p - tsato its base ( e - pcz ) , sem images ( figure 5(e ) ) show only porous structure with small pores of size ( 0.5 to 1  m ) and higher pores of size ( 5 to 6.5  m ) , whereas sem images of s - pcz - p - tsa ( figure 5(f ) ) and its corresponding base ( figure 5(g ) ) show flake - like structure . x - ray diffraction profiles registered for polycarbazole samples , s - pcz - p - tsa , s - pcz , e - pcz - p - tsa , and e - pcz , are shown in figure 2 . x - ray diffraction patter of s - pcz - p - tsa showed three broad peaks around 2 = 6 , 18 , and 27 with corresponding d - spacing 16.7 , 5.1 , and 3.3 , respectively ( figure 6(a ) ) , whereas pcz samples of s - pcz , e - pcz - p - tsa , and e - pcz showed two very broad bands around 6 to 8 and 18 to 23 ( figures 6(b)6(d ) ) . x - ray results of pcz salts and bases prepared in the present work show amorphous nature . tga thermograms of polycarbazole samples are recorded from ambient temperature to 700c under nitrogen atmosphere and are shown in figure 7 . its base ( s - pcz ) , and e - pczshows that these samples are stable up to 110c . however , polycarbazole sample prepared by emulsion polymerization pathway ( e - pcz - p - tsa ) is stable up to 200c . s - pcz - p - tsa powder sample was pressed on stainless steel mesh and used as working electrode for cv measurement . cv of s - pcz - p - tsa polymer electrode was carried out in acetonitrile using 0.1  m tetraethylammonium tetrafluoroborate as supporting electrolyte at a scan rate 10  mv / s with ag / agcl reference electrode in single one cycle . cv of s - pcz - p - tsa shows one redox peak , anodic peak at 0.9  v , and cathodic peak at 0.74  v ( figure 8) , which justifies the formation of the polymer . a similar result was observed for polycarbazole prepared by interfacial pathway using ammonium persulfate oxidant by gupta and prakash . however , the electroactive nature of s - pcz - p - tsa sample is less and this may be due to overoxidation ( overoxidation is supported by infrared spectrum ) . benzoyl peroxide has been demonstrated as oxidizing agent in the oxidation of carbazole to solvent soluble polycarbazole . polycarbazole salt prepared by solution polymerization pathway was obtained in semiconductor range ( 1.5  10  s / cm ) with density ( 1.15  g / cm ) and reasonable yield ( 69  wt% with respect to the amount of carbazole used ) . polycarbazole salts prepared by both solution ( ~10 repeating units ) and emulsion polymerization pathways ( ~12 repeating units ) were soluble in less and high polar solvents . moreover , polycarbazole salt prepared by emulsion polymerization pathway was also soluble in chloroform . polycarbazole salt prepared by emulsion polymerization pathway shows mixture of shapes with microrod ( 830  m of length and 2.5  m of width ) , sphere ( 3 to 7  m diameter ) , and pores ( 0.6 to 1.1  m ) . its corresponding base shows only micropores of size 0.5 to 6.5  m , whereas polycarbazole salt and its corresponding base prepared by solution polymerization pathway show flake - like morphology . higher thermal stability was obtained for polycarbazole salt prepared by emulsion polymerization pathway than that of the salt prepared by solution polymerization pathway . this polycarbazole powder will be useful for coating and making antistatic films with common insulating polymers .
carbazole was oxidized by benzoyl peroxide in presence of p - toluenesulfonic acid to polycarbazole salt at room temperature for the first time . 
 polycarbazole salts were synthesized via solution and emulsion polymerization pathways . 
 polycarbazole bases were prepared by dedoping from polycarbazole salts . 
 formation of polycarbazoles was confirmed from infrared , electronic absorption and edax spectra . 
 polycarbazole salt was obtained in amorphous nature in semiconductor range ( 105  s / cm ) , which was found to be soluble in less and high polar solvents . 
 polycarbazole salt prepared by emulsion polymerization pathway showed mixture of shapes with microrod , sphere , and pores , whereas its corresponding base showed only micropores structure . on the other hand , polycarbazole salt and 
 its corresponding base prepared by solution polymerization pathway showed flake - like morphology . 
 higher thermal stability was obtained for polycarbazole salt prepared by emulsion polymerization pathway than that of the salt prepared by solution polymerization pathway .